LMucko/crystallography-open-database huggingface dataset:
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517921
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47281(14)
_cell_length_b                   7.47281(14)
_cell_length_c                   7.47281(14)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    120
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.303(14)
_diffrn_ambient_temperature      120
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2535(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.58
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.21
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.80
_refine_ls_R_I_factor            1.09
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_120K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.30(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517921
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517922
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47607(16)
_cell_length_b                   7.47607(16)
_cell_length_c                   7.47607(16)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.850(15)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2480(3)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.73
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.23
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.82
_refine_ls_R_I_factor            1.05
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_300K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.85(3)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517922
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517923
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47450(17)
_cell_length_b                   7.47450(17)
_cell_length_c                   7.47450(17)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    240
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.586(16)
_diffrn_ambient_temperature      240
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2507(3)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.63
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.14
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.74
_refine_ls_R_I_factor            1.03
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_240K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.59(3)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517923
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517924
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47260(12)
_cell_length_b                   7.47260(12)
_cell_length_c                   7.47260(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    20
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.268(12)
_diffrn_ambient_temperature      20
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2538(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.63
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.21
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.80
_refine_ls_R_I_factor            1.19
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_20K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.269(19)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517924
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517925
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47266(11)
_cell_length_b                   7.47266(11)
_cell_length_c                   7.47266(11)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    5
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.278(11)
_diffrn_ambient_temperature      5
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2537(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.64
_pd_proc_ls_prof_wR_expected     1.12
_pd_proc_ls_prof_wR_factor       7.22
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.80
_refine_ls_R_I_factor            1.17
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_5K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.279(19)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517925
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517926
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47268(15)
_cell_length_b                   7.47268(15)
_cell_length_c                   7.47268(15)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    100
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.282(15)
_diffrn_ambient_temperature      100
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2537(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.60
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.20
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.78
_refine_ls_R_I_factor            1.05
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_100K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.28(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517926
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517927
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47262(14)
_cell_length_b                   7.47262(14)
_cell_length_c                   7.47262(14)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    80
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.271(14)
_diffrn_ambient_temperature      80
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2538(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.61
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.22
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.80
_refine_ls_R_I_factor            1.12
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_80K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.27(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517927